SUPERSEDED (click for Active standard)
| ||Format||Pages||Price|| |
|10||$52.80||  ADD TO CART|
1.1 This test method describes a procedure for conducting stress-corrosion cracking tests in an acidified boiling sodium chloride solution. This test method is performed in 25% (by mass ) sodium chloride acidified to pH 1.5 with phosphoric acid. This test method is concerned primarily with the test solution and glassware, although a specific style of U-bend test specimen is suggested.
1.2 This test method is designed to provide better correlation with chemical process industry experience for stainless steels than the more severe boiling magnesium chloride test of Practice G36. Some stainless steels which have provided satisfactory service in many environments readily crack in Practice G36, but have not cracked during interlaboratory testing using this sodium chloride test method.
1.3 This boiling sodium chloride test method was used in an interlaboratory test program to evaluate wrought stainless steels, including duplex (ferrite-austenite) stainless and an alloy with up to about 33% nickel. It may also be employed to evaluate these types of materials in the cast or welded conditions.
1.4 This test method detects major effects of composition, heat treatment, microstructure, and stress on the susceptibility of materials to chloride stress-corrosion cracking. Small differences between samples such as heat-to-heat variations of the same grade are not likely to be detected.
1.5 The values stated in SI units are to be regarded as the standard. The values given in parentheses are for information only.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. For specific hazard statements, see Section 7.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D1193 Specification for Reagent Water
E8 Test Methods for Tension Testing of Metallic Materials
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
G15 Terminology Relating to Corrosion and Corrosion Testing
G16 Guide for Applying Statistics to Analysis of Corrosion Data
G30 Practice for Making and Using U-Bend Stress-Corrosion Test Specimens
G36 Practice for Evaluating Stress-Corrosion-Cracking Resistance of Metals and Alloys in a Boiling Magnesium Chloride Solution
G49 Practice for Preparation and Use of Direct Tension Stress-Corrosion Test Specimens
G107 Guide for Formats for Collection and Compilation of Corrosion Data for Metals for Computerized Database Input
ICS Number Code 77.060 (Corrosion of metals)
UNSPSC Code 41114604(Corrosion testers)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM G123-00(2005), Standard Test Method for Evaluating Stress-Corrosion Cracking of Stainless Alloys with Different Nickel Content in Boiling Acidified Sodium Chloride Solution, ASTM International, West Conshohocken, PA, 2005, www.astm.orgBack to Top